Master Degree Project

Department of Transport Science

Royal Institute of Technology

Thermal Cracking Model

School of Architecture and the Built Environment

Royal Institute of Technology (KTH)

SE- 100 44 Stockholm

[email protected]
Abstract: Low temperature cracking is an important form of asphalt
pavement deterioration in cold regions. The cracks develop when
thermally induced stresses exceed the fracture resistance of the
asphalt pavement. In this study, by incorporating HMA fracture
mechanics into thermal cracking model, a new integrated model is
introduced to investigate low temperature cracking performance. To
evaluate its reliability and accuracy, the predicted thermally
induced stress and failure temperature are compared with the
fracture stress and fracture temperature obtained from thermal
stress restrained specimen test. The findings indicate that this
HMA fracture mechanics-based thermal cracking model has a great
potential to reliably evaluate the performance of asphalt mixtures
subjected to thermally induced damage.

KEY WORDS: Hot Mix Asphalt; Low temperature cracking; HMA fracture
mechanics; Thermal cracking model; SuperPave IDT; Thermal Stress
Restrained Specimen Test

ii

iii

Acknowledgement

First of all, I would like to sincerely thank my thesis advisor at
Royal Institute of Technology (KTH), Dr. Denis Jelagin, for his
professional expertise and patient guidance. I am honored and very
grateful that I could study and research under his supervision. For
me, Dr. Jelagin is not only an eximious academic expert and
advisor, but also a great moral and ethical model. Without his
invaluable instruction I would not finish my degree.

I would express my special thanks to Mr. Prabir Kumar Das, whose
research on fracture mechanics of asphalt pavement greatly
supported my thesis project. I sincerely appreciate him for his
expert guidance, especially during the whole process of the tests.
Working with him in Asphalt Laboratory gave me a lot of edification
and fulfillment.

Also I wish to thank Dr. Michael Behn and other PhD students in the
Division of Highway and Railway Engineering who helped me during my
thesis project work, for their great advices and supports.

Finally, I owe my sincere gratitude to all my classmates and
friends who accompany me during this two-year master program.

iv

v

List of Symbols

ai Half of crack length ag Slope of lower asymptote al Slope of
higher asymptote C Crack depth C0 Current crack length Ccomp
Non-dimensional creep compliance factor Cr Creep compliance Csx
Horizontal stress correction factor C Constant without physical
significance d Diameter of specimen D Thickness of asphalt pavement
surface layer D0 Creep compliance parameter D1 Creep compliance
parameter D(ξ) Creep compliance at reduced time ξ D(ξ − ξ′) Creep
compliance at reduced time ξ-ξ′ DCSEf Dissipated Creep Strain
Energy to failure DCSEmin Minimum Dissipated Creep Strain Energy Ei
Prony series parameter E(ξ) Relaxation modulus at reduced time ξ
E(ξ − ξ′) Relaxation modulus at reduced time ξ-ξ′ GL Gauge length h
Thickness of specimen L[D(t)] Laplace transform of creep compliance
L[E(t)] Laplace transform of relaxation modulus m Creep compliance
parameter MR Resilient modulus n Number of Kelvin elements N Number
of loading cycle Pen77 Penetration value at 770F (250C) r Distance
from crack tip R Parameter representing the curve between
asymptotes P Load s Laplace parameter S Cracks spacing of asphalt
pavement surface layer St Tensile strength tDCSE Time to 5 mm crack
length Due to Dissipated Creep Strain Energy tFE Time to 5 mm crack
length Due to Fracture Energy

vi

T Temperature Tg Glass transition temperature (ξ′) Temperature
change rate St Tensile strength t Time X/Y Ratio of horizontal to
vertical deformation α Thermal contraction coefficient αT Time -
temperature shift factor εf Failure strain ε() Thermal strain at
reduced time ξ εcr() Thermal creep strain at reduced time ξ ε(ξ′)
Thermal strain rate η Binder viscosity λi Prony Series parameter ν
Poisson’s Ratio ξ Reduced time ξ′ Real time integrating variable σ
Stress σAVG Average stress σFA Faraway stress from pavement σ(ξ)
Stress at reduced time ξ τ Prony series parameter υ Specific volume
change ΔH Horizontal deformation ΔS/ΔT Slope of stress-temperature
curve of Thermal Stress Restrained Specimen Test

vii

List of Abbreviations

AASHTO - American Association of State Highway and Transportation
Officials ABT - Allmän Teknisk Beskrivning (General Technical
Standards) CCMC - Creep Compliance Master Curve DCSE - Dissipated
Creep Strain Energy ESALs - Equivalent Single Axle Load EE -
Elastic Energy ER - Energy Ratio FE - Fracture Energy HMA - Hot Mix
Asphalt IDT - Indirect Tensile Test LVDT - Linear Variable
Differential Transducer NCHRP - National Cooperative Highway
Research Program SHRP - Strategic Highway Research Program TCMODEL
- Thermal Cracking Model TSRST - Thermal Stress Restrained Specimen
Test

viii

ix

1. Introduction …………………………………………………………………………….. 1 2. HMA Fracture
Mechanics ……………………………………………………………... 3

2.1 Fracture Thresholds …………………………………………………………………. 3 2.2 Crack
Growth Law …………………………………………………………………... 4 2.3 Energy Ratio
………………………………………………………………………… 5

3. HMA Fracture Mechanics-Based Thermal Cracking Model ……..…………………
7 3.1 Thermal Cracking Performance Model ……………………………………………...
7

3.1.1 Thermal Cracking Mechanism ……………………………………………... 7 3.1.2 Crack
Propagation Model …………………………………………………... 8

3.2 Thermal Cracking Prediction ………………………………………………………... 8 3.2.1
Thermal Contraction Coefficient …………………………………………… 9 3.2.2 Creep
Compliance Master Curve …………………………………………… 9 3.2.3 Conversion of
Creep Compliance to Relaxation Modulus ………………... 10 3.2.4
Calculation of Thermal Stress …………………………………………….. 11

3.3 General Concept of HMA Fracture Mechanics-Based Thermal
Cracking Model … 12 3.3.1 Calculation of Dissipated Creep Strain
Energy …………………………… 13 3.3.2 Calculation of Fracture Energy
……………………………………………. 15 3.3.3 Calculation of Crack Length
………………………………………………. 15

4. Experimental Design ………………………………………………………………….. 16 4.1 Sample
Preparation ………………………………………………………………… 16 4.2 SuperPave IDT
……………………………………………………………………... 18

4.2.1 Resilient Modulus Test ……………………………………………………. 18 4.2.2 Creep
Compliance Test ……………………………………………………. 19 4.2.3 Tensile Strength
Test ……………………………………………………… 19

4.3 Thermal Stress Restrained Specimen Test ………….………………………………
20

5. Data Analysis ………………………………………………………………………….. 22 5.1 SuperPave
IDT and TSRST Data ………………………………………………….. 22 5.2 Creep Compliance
Master Curve and Relaxation Modulus ……………………….. 23 5.3 Thermally
induced Stress with Constant Thermal Contraction Coefficient ………..
28 5.4 Fracture Temperature ………………………………………………………………. 35 5.5 Effect
of Thermal Contraction Coefficient ………………………………………… 36

6. Summary and Conclusion …………………………………………………………….. 39 References
………………………………………………………………………………….. 41
Appendix……………………………………………………………………………………. 43

x

1

1. Introduction

The common distress of asphalt pavement in cold regions is the low
temperature cracking, which results from the contraction and
expansion of the asphalt pavement under extreme temperature changes
(Birgisson et al., 2004). Generally it appears as regularly spaced
transverse cracks across pavement surface as shown in Figure 1.
Water entering the crack may freeze during wintertime and result in
the formation of ice lenses, which in turn may produce frost heave.
Pumping of fines through the crack may produce voids under the
pavement, which means that the bearing capacity may be reduced.
Consequently, the low temperature cracking may cause poor ride
quality, reduce service life and increase costs for rehabilitation.
Recently, a Hot Mix Asphalt (HMA) fracture mechanics-based thermal
cracking model was developed by Das et al. (2011). In this project,
the susceptibility of asphalt mixtures to low temperature cracking
will be studied by this model which incorporates a fundamental
crack growth mechanism associated with damage accumulation and the
dissipated energy threshold.

Figure 1. Typical Thermal Cracking in Asphalt Pavement

The principal objective of this project is to evaluate the HMA
fracture mechanics-based thermal cracking model. The work comprises
the following subtasks:

i. Reviewing the energy-based HMA fracture mechanics and the
Thermal Cracking performance Model (TCMODEL).

ii. Implementing the HMA fracture mechanics-based thermal cracking
model with the experimental input data.

2

iii. Validating the predicted thermally induced stress and fracture
temperature with the Thermal Stress Restrained Specimen Test
(TSRST).

In experimental design, the SuperPave InDirect Tension Tests
(SuperPave IDT) are conducted to collect the mechanical properties
of three design asphalt mixtures, which serve as the input
parameters in the HMA fracture mechanics-based thermal cracking
model. Then first the model generates Creep Compliance Master Curve
(CCMC) to obtain creep compliance. By converting the creep
compliance to relaxation modulus, the model in turn calculates
thermal stress and creep strain. Based on energy principle, the
total accumulated Dissipated Creep Strain Energy (DCSE) and the
total accumulated Fracture Energy (FE) govern the crack development
until failure. Finally the model outputs the thermal stress with
the changing temperatures and gives an accurate prediction as crack
length versus temperature or time.

With different binder grades (Pen77 35/50, 70/100 and 160/220), in
total 27 core specimens (150 mm in diameter and 50 mm in thickness)
are tested by SuperPave IDT at different temperatures (0 °C, -10 °C
and -20 °C), respectively. Also each 4 beam specimens (38 mm × 38
mm × 200 mm) with the same 3 binder grades as SuperPave IDT are
tested by TSRST. The predicted thermal stress and fracture
temperature are compared with the corresponding values obtained
from the TSRST to evaluate the reliability and accuracy of the
model.

3

2. HMA Fracture Mechanics

Cracking mechanism in asphalt mixture may be better understood with
the theory of fracture mechanics which combines the mechanics of
crack initiation or propagation with the mechanical properties of
material. An HMA fracture mechanics model developed by Zhang et al.
(2001) at University of Florida provided a fundamental crack growth
law for evaluating performance of asphalt mixture. The HMA fracture
mechanism primarily consists of two principal theories: theory of
linear viscoelasticity and energy-based fracture mechanics. The
following sections provide an explanation of the basic principles
of HMA fracture mechanics.

2.1 Fracture Thresholds

The fundamental fracture threshold is the core of the HMA fracture
mechanics model presented by Zhang et al. (2001). The concept is
based on the observation of the discontinuous crack growth in HMA
material (Figure 2). Micro-damage (i.e. the damage which does not
result in crack initiation or growth) appears to be fully healable,
while macro-damage (i.e. the damage which results in crack
initiation or growth) does not appear to be healable.

Figure 2. Crack Propagation in Asphalt Mixture (Birgisson et al.,
2004)

The macro-damage development at any time during either crack
initiation or propagation is mastered by the lower and upper
thresholds: Dissipated Creep Strain Energy to failure (DSCEf) and
Fracture Energy (FE). Accordingly, Birgisson et al. (2007)
suggested two possibilities that the macro-damage develops in
asphalt mixture. One is due to creep strain energy, a number of
continuously repeated loads with stresses significantly below the
tensile strength would cause damage accumulation and lead to
fracture when the DSCEf is reached. The other way is when any large
single load applied during the loading cycle exceeds the

4

FE threshold then fracture would occur.

DSCEf has been found to be independent of loading mode or loading
history. Therefore, the development of crack in asphalt mixture can
be determined by calculating the amount of DSCE induced by any
loading condition and comparing it to the DSCEf of the asphalt
mixture. As illustrated in the stress-strain response (Figure 3),
DSCE is determined by the difference between FE and Elastic Energy
(EE) for a single load. FE is the area under stress-strain curve to
the failure strain.

Figure 3. Graphical Illustration of DCSE (Birgisson et al.,
2004)

2.2 Crack Growth Law

Based on the concept of energy threshold, Zhang et al. (2001)
developed the HMA fracture mechanics model. It was assumed to have
a 10 mm initial crack size based on the typical aggregate size of
asphalt mixtures. According to Birgisson et al. (2007), the
continuous cyclic loading will increase the accumulative DCSE in
the initiation zone until it reaches the DCSE threshold as showed
in Figure 4a. Then the stress at the crack tip will draw a high
rate of DCSE accumulation in the process zone next to the crack tip
(Figure 4b). The length of the process zone γi is defined by
Equation [1].

γi = 1 2 σFA

St 2 ai (i > 1) [1]

where St is tensile strength, σFA is faraway stress and ai is
current crack length. In Figure 4c, the DCSE accumulation process
continues in the new process zone and the crack grows at a faster
rate in the new process zone.

5

Figure 4. Crack Growth Process in HMA Fracture Mechanics Model
(Birgisson et al., 2007)

2.3 Energy Ratio

Roque et al. (2004) introduced Energy Ratio (ER) into the HMA
fracture mechanics model to further evaluate the fracture
performance of asphalt mixture. ER is defined as DCSEf of asphalt
mixture over DCSEmin which is the minimum DCSE required for a good
cracking performance that serves as a single criterion for cracking
performance by considering both asphalt mixture properties and
pavement characteristics. ER is a measure of fracture resistance of
asphalt mixture and can be calculated as follow:

ER = DCSEf DCSEmin

[2]

where DCSEf is dissipated creep strain energy to failure, DCSEmin
is minimum dissipated creep strain energy for adequate cracking
performance and St is tensile strength. DSCEmin is a function of
creep compliance power law parameters (m-value and D1) as
illustrated in Figure5. For a good field performance of the
mixture, the ER should be greater than 1.0.

The basic principles of HMA fracture mechanics are shown in Figure
6 if two asphalt mixtures with different properties are compared.
For either asphalt mixture, the DCSE increases with number of load
applications (ESALs). The asphalt mixture with higher creep

6

compliance power law (m-value and D1) exhibits a higher rate of
dissipated creep strain energy accumulation. However, this does not
necessarily imply that cracks will initiate or propagate more
quickly in this asphalt mixture, as it depends on the energy
threshold, which varies significantly between asphalt mixtures and
is not necessarily related to its creep characteristics.

Figure 5. Creep Compliance Power Law Parameters (Roque et al.,
2004)

Figure 6. Basic Principles of HMA Fracture Mechanics Model (Roque
et al., 2004)

It is evident that no single asphalt mixture property can be used
to predict asphalt mixture cracking performance reliably. In order
to use the HMA fracture mechanics-based thermal cracking model,
resilient modulus (M), creep compliance power law parameters
(m-value and D1), tensile strength (St), dissipated creep strain
energy to failure (DCSEf) and Fracture Energy (FE) are required.
More details about how to obtain all these parameters from the
SuperPave IDT were specified by Du (2010).

7

3. HMA Fracture Mechanics-Based Thermal Cracking Model

Low temperature cracking is a thermally induced distress caused by
the extremely temperature change in cold climate. The existence of
transverse cracks eventually causes thermal contraction and
failure, resulting in different kinds of degradation to asphalt
pavement. Several different thermal cracking models have been
developed by applying empirical and/or analytical methods. Few of
them, however, attempt to incorporate a fundamental crack growth
mechanism associated with damage accumulation and the dissipated
energy threshold in asphalt pavement. Therefore, a mechanics-based
thermal cracking performance model, which is able to incorporate
the energy-based HMA fracture mechanics, may provide a proper
framework to evaluate the thermal cracking performance of asphalt
pavement.

3.1 Thermal Cracking Performance Model

As part of the Strategic Highway Research Program (SHRP), a
mechanics-based Thermal Cracking performance Model (TCMODEL,
Hiltunen and Roque, 1994) was developed based on the theory of
linear viscoelasticity. TCMODEL predicts the amount of thermal
cracking that will develop in an asphalt pavement as a function of
time, which provides the basis for a true performance-based mixture
specification for thermal cracking.

3.1.1 Thermal Cracking Mechanism

The thermal contraction strains induced by pavement cooling always
lead to thermal tensile stress development in the restrained
surface layer. On the other hand, the tensile strength of asphalt
pavement increases only to a maximum and then decreases. Thermal
tensile stress development is mostly in the longitudinal direction
of pavement since this direction is restrained. Also thermal
tensile stress is greatest at the surface of pavement because of
the lower temperature and the higher temperature change (Witczak et
al. 2000). In Figure 7, an asphalt pavement surface layer of
thickness D is shown to be subjected to a tensile stress
distribution with depth and the potential crack sites are uniformly
spaced at a distance S.

There are two different types of thermal cracking. In case of very
severe cooling cycles, e.g. extremely low temperature and/or fast
cooling rates, low-temperature cracking may occur when the thermal
tensile stress in asphalt mixture exceeds its tensile strength. If
the tensile stress is below the tensile strength, the pavement will
not crack under a single daily temperature cycle but could still
crack after a long time tensile stress accumulation. This is
usually referred to as thermal fatigue cracking. Essentially the
failure mechanisms are same for these two types of cracking and the
only difference is the rates at which cracks occur.

8

Figure 7. Physical Model of Asphalt Pavement (Witczak et al.,
2000)

3.1.2 Crack Propagation Model

Temperature-induced thermal cracking is a “top-down” initiation and
propagation. During the cooling process, stresses develop due to
the contraction of asphalt pavement. The stresses are not constant
with depth because of a thermal gradient in the pavement and the
temperatures vary with the depth. Within the surface layer there
are potential crack zones uniformly spaced at a regular distance
(Figure 7). At each of these crack zones the thermally induced
stresses can cause a crack to propagate through the surface layer
(Figure 8), where ΔC is the crack growth due to the cooling cycle
and C0 is the initial crack length for the next cooling cycle. Due
to spatial variation of the relevant material properties within the
surface layer, each of these cracks can propagate at a different
rate (Witczak et al. 2000).

Figure 8. Crack Depth Fracture Model (Witczak et al., 2000)

3.2 Thermal Cracking Prediction

The physical behavior of asphalt mixture can be approximated by
theory of linear viscoelasticity. It exhibits viscosity even at low
temperature which will affect the thermal cracking performance of
an asphalt pavement.

9

i. Gathering input data and introducing them into the
TCMODEL.

ii. Developing Creep Compliance Master Curve (CCMC).

iii. Converting creep compliance to relaxation modulus.

iv. Predicting thermal stress using viscoelastic transformation
theory.

3.2.1 Thermal Contraction Coefficient

Thermal contraction coefficient (α) is one of the thermo-mechanical
properties required in the prediction of thermal cracking of
asphalt pavements because thermally induced stresses and strains
are directly proportional to it. The α value of asphalt mixture is
dependent on the thermal properties of selected binder and mineral
aggregate.

Although the thermal contraction coefficient of asphalt mixture has
non-linear behavior, a simplified α value (constant, linear or
bi-linear) has been using in many thermal cracking models. The
reliability of thermal cracking prediction is mostly depends upon
the accuracy of this value. In this study, the constant thermal
contraction coefficients obtained from stress-temperature curve of
TSRST are applied. Alternatively, the non-linearity of thermal
contraction coefficient is taken into account while calculating
thermally induced stresses and strains by using the following
Equations developed by Nam and Bahia (2004):

α = dυ dT

[3]

υ = cv + agT − Tg + Ral − agln 1 + exp (T−Tg) R

[4]

where υ is specific volume change in ml/g; cν is a constant without
physical significance; Tg is glass transition temperature; ag and
al is slope of lower and higher asymptote

respectively and R is a parameter representing the curvature
between asymptotes. More information about how to apply the
no-linear thermal contraction coefficient on the same three design
asphalt mixtures was specified by Das et al. (2011).

3.2.2 Creep Compliance Master Curve

Since the viscoelastic properties of asphalt mixture are
temperature dependent, the model requires creep compliance
parameters (D0, D1 and m-value) at three different temperatures (0
°C, -10 °C and -20 °C). These parameters can be determined from the
SuperPave IDT

10

static creep test. Whereas, creep compliance is simply the time
independent stain divided by the constant stress used in the creep
test. Once the parameters are known, Creep Compliance Master Curve
(CCMC) can be generated by using time-temperature superposition
principle (Hiltunen and Roque 1994; Buttlar et al. 1998). The
lowest temperature (-20 °C) is set as reference temperature. Then
as showed in Figure 9, the CCMC is fitted with power model in
log-log scale and mathematically it can be expressed as follow
(Witczak et al. 2000):

D(ξ) = D0 + D1ξm [5]

where D(ξ) is creep compliance at reduced time ξ and D0 , D1 and m
are the creep compliance parameters. In chapter 5 Figures (17 -
22), the different creep compliance data and the CCMC fitted by
power law for each of the three design asphalt mixtures are
illustrated, respectively.

Figure 9. Power Model of Creep Compliance (Witczak et al.,
2000)

3.2.3 Conversion of Creep Compliance to Relaxation Modulus

Since creep and stress relaxation phenomena are two aspects of the
same viscoelastic behavior of material, they are obviously related.
The relationship between creep compliance and relaxation modulus
can be presented by a convolution integral as follows:

∫ D(t − ξ) dE(ξ) dξ

∞ 0 dξ = 1 [6]

Applying the Laplace transformation to Equation [6] then yield
Equation [7],

L[D(t)] L[E(t)] = 1 S2

[7]

where L[D(t)] is Laplace transformation of the creep compliance,
L[E(t)] is Laplace transformation of the relaxation modulus, s is
the Laplace parameter and t is time (for the master curve, the
reduced time ξ is used).

11

Once the relaxation modulus is known, it can be presented by a
generalized Maxwell model to represent the viscoelastic properties.
Mathematically, the relaxation modulus for a generalized Maxwell
model can be expressed according to the following Prony
Series.

E(ξ) = ∑ Eie−ξ/λiN+1 i=1 [8]

where E(ξ) is relaxation modulus at reduced time, Ei and λi are the
Prony series parameters for relaxation modulus master curve. In
chapter 5 Figures (23 - 25), the relaxation modulus fitted by Prony
Series for each of the three design asphalt mixtures are
illustrated, respectively.

3.2.4 Calculation of Thermal Stress

For transient temperature conditions where the temperature varies
with the time, thermal stress is generally involved and developed
due to the thermal contraction. For linear viscoelastic materials,
the thermal stress can be predicted by using Boltzmann’s
Superposition Principle.

σ(ξ) = ∫ E(ξ − ξ′) dε(ξ′) dξ′

ξ 0 dξ′ [9]

where σ(ξ) is the stress at reduced time ξ, E(ξ − ξ’) is relaxation
modulus at reduced time and ξ′ is the real time integrating
variable. Morland and Lee (1960) introduced the following reduced
time, which is able to take into account both effects of
temperature gradients and time variations coincidently.

ξ(t) = ∫ 1 αT(T(t′))

dt′t 0 [10]

where αT is the time-temperature shift factor which can be
determined from Arrhenious Equation or Williums-Landel-Ferry (WLF)
Equation.

The other parameter thermal strain rate ε(ξ′) [i.e. (′) ′

] which is directly related to the

thermal contraction coefficient ().

Where the rate of change in temperature T(ξ′) = dT(ξ′)/dξ′.

12

3.3 General Concept of HMA Fracture Mechanics-Based Thermal
Cracking Model

The general concept used to calculate the amount of crack
development of the HMA fracture mechanics-based thermal cracking
model consists of 5 steps:

i. Defining the process zones.

ii. Predicting thermal stress.

iv. Calculating and assigning DCSE within each individual process
zone.

v. Calculating and assigning FE within each individual process
zone.

The number of process zones contributes as an important factor that
affects the computation time. In this model, a 10 mm initial crack
length followed by 5 mm of processing zone is assumed, which
generally corresponds to half the nominal maximum aggregate size.
Also a 100 mm crack limit is set, so the program is automatically
stopped when the total length of crack reaches 100 mm.

The procedure of thermal stress prediction has been discussed in
section 3.2.4. In each process zone, an average value of the
thermally induced tensile stress is calculated at small time
increments. These average values are subsequently used to calculate
the DCSE and FE over the process zone. The details of DCSE and FE
calculations for each process zone are presented in the following
sections. An overall flow chart for crack development calculation
of HMA fracture mechanics-based thermal cracking model is
illustrated as Figure 10.

13

No

Total Crack ≥ 100mm

Crack length vs. Time (or Temp.)

Calculate: DCSE for Each Zones and Transfer DCSE to Reference
Temperature

Calculate: FE for Each Zones and Transfer FE to Reference
Temperature

DCSE ≥ DCSE limit FE ≥ FE limit

tDCSE (time to crack 5mm) tFE (time to crack 5mm)

Input: D0,D1, m, DCSE limit, FE and Tensile

Input: Thermal Contraction Coefficient, Cooling Rate

Define Processing Zone

Calculate: Shift factor, Prony Series Parameters for Relaxation
Modulus

Calculate: Thermal Stress, Creep strain and Thermal strain

Figure 10. General Steps of HMA Fracture Mechanics-Based Thermal
Cracking Model (Das et al., 2011)

14

3.3.1 Calculation of Dissipated Creep Strain Energy

Viscoelastic materials subjected to a step constant stress
experience a time-dependent increase in strain. This phenomenon is
known as viscoelastic creep and the time-dependent total strain
produced by applied stress is known as creep strain.

Although the power model has been successfully used as a fitting
function of the creep behavior for linear viscoelastic materials,
its mathematical deficiency does not allow predicting the thermal
stress of viscoelastic materials under multiple temperature ranges.
In SHRP A-005 study, the thermal creep strain was predicted by
viscosity ην obtained from the Prony series (Generalized
Voight-Kelvin model) (Buttlar et al. 2009).

D(ξ) = D0 + ∑ 1 − e − ξ τi+ ξ

ην n i=1 [12]

where D(ξ) is the creep compliance at reduced time ξ; D0 , D1 , τi
are Prony series parameters and n is the number of Kelvin elements.
The presence of viscous flow at long loading times can be presented
by ην which is the viscosity as ξ → ∞. Considering only the viscous
component representing the rate of damage of viscoelastic media,
Equation [12] can be simplify as

D(ξ) = ξ ην

[13]

The thermal creep strain εcr can be predicted from time-temperature
constitutive strain Equation [15] combining with irreversible creep
component ην.

ε(ξ) = ∫ D(ξ − ξ′) dσ(ξ′) dξ′

ξ 0 dξ′ [14]

dξ′ dξ′ [15]

where ε(ξ) is the stain at reduced time ξ, D(ξ − ξ’) is creep
compliance at reduced time and ξ′ is the real time integrating
variable.

The thermal strain resulting from the tensile stress is
irreversible. The dissipated creep strain energy (DCSE) is an
irreversible parameter representing fundamental energy loss in
viscoelastic materials, which generally can be determined from the
thermal stress and creep strain relationship. Therefore, DSCE can
be obtained at each time increment if the thermal stress and
thermal creep strain are known. It may be more convenient to detect
the failure if the DCSEf are same at any temperature. However in
reality, DCSEf is constant at fixed temperature but it may vary
with changing temperature. Based on energy principle, DCSE at

15

small time increment (t) can be determined by transferring DCSEf at
the reference temperature using the following equation (Kim et al.
2008):

DCSE(t) = σ(t)−σ(t−t) 2

εcr(t) − εcr(t− t) DCSEf at Reference Temperature DCSEf at Given
Temperature

[16]

So total accumulated DCSE can be obtained from the summation of
DCSE at each time increment.

DCSE(t) = ∑DCSE(t) [17]

3.3.2 Calculation of Fracture Energy

Fracture Energy (FE) is another threshold which develops due to the
temperature change in the pavement. The area under the thermally
induced stress-strain curve is known as fracture energy. The
calculated average stresses over the process zones calculated by
the thermal stress at small time increments are used to get the FE
over the process zone. As FE limits are changing with the
temperature change so FE limits at the given temperature should be
transferred to a correspondent FE limit at a reference temperature
as follow (Kim et al. 2008):

FE(t) = ∫ σAVG(t)ε(t)dtt 0 FE at Reference Temperature

FE at Given Temperature [18]

3.3.3 Calculation of Crack Length

Once the DCSE and FE are obtained then assigned to each process
zone. The process zone near the crack tip is failed once the total
accumulated DCSE reaches DCSEf or the total accumulated FE reaches
FE limit. At the same time as the crack length is increasing so the
stress distribution along the process zone is also changing. Then
in the next step the stress redistributes along the processing
zone. This iteration process continues until the crack length
reaches total 100 mm.

16

4 Experimental Design

A series of the SuperPave InDirect Tension Test (SuperPave IDT) and
the Thermal Stress Restrained Specimen Test (TSRST) are conducted
in this experimental design. The details of raw materials, sample
preparations and test introductions are presented in the following
sections. All the results from each type of tests then are followed
in Chapter 5 for the data analytical studies.

4.1 Sample Preparation

In these tests, three dense graded asphalt mixtures with different
binders (Pen77 35/50, 70/100 and 160/220) are prepared according to
ATB 11 of the Swedish Road Standards (ABT VÄG 2004). The aggregates
consisted of a crushed granite from Skäalunda Quarry in Sweden with
the maximum size of 11 mm are selected. The aggregate graduation
used to prepare the design asphalt mixtures is shown in Table 1 and
Figure 11. The 3 binders with different penetration grades are used
in these tests. The softening point (EN 1427) and penetration at 25
°C (EN 1426) were measured and given in Table 2.

Table 1. Aggregate Gradation Design

Sieve Size Targeted Gradation Selected Gradation mm % % 22.4 100
100 100 100 16 98 100 99 100

11.2 85 99 92 91.2 8 70 88 79 80.9

5.6 58 75 66.5 66.9 4 48 66 57 59.0 2 33 52 42.5 43.5 1 23 42 32.5
31.3

0.5 16 31 23.5 22.6 0.25 11 22 16.5 16.2

0.125 8 15 11.5 11.5 0.063 6 9 7.5 6.3

Specification Limits %

Table 2. Properties of Binders

Properties Units

Penetration dmm 45 81 185

The aggregates and binders to be mixed are preheated at mixing
temperature 155 °C for 3 hours and 1.5 hours, respectively. The
compaction temperature is 135 °C. The normal binder content is 6.2%
by mass and the air void is 2 ± 0.5% by volume. The slabs are
produced by using gyratory compactor (Model ICRT-150R/RB). The
compacted slabs denoted as Mix-35-50, Mix-70-100 and Mix-160-220
are extruded from moulds and cool at room temperature for 24
hours.

For each design asphalt mixture, 9 cylindrical specimens (150 mm in
diameter and 50 mm in thickness) are extracted for SuperPave IDT
and 4 beam specimens with 38mm × 38mm × 200mm are sawed for TSRST,
respectively. When preparing IDT specimens, it is significantly
important to enable a smooth surface for mounting gage
points.

0

20

40

60

80

100

% p

4.2 SuperPave IDT

As a part of the Strategic Highway Research Program (SHRP) (NCHRP,
2004), the SuperPave IDT was developed to determine resilient
modulus (MR), creep compliance (Cr), m-value, D1, tensile strength
(St), failure strain (σ), fracture energy (FE) and dissipated creep
stain energy to failure (DCSEf). It consists of resilient modulus,
creep compliance and tensile strength tests.

In this study, these tests were performed at 0 °C, -10 °C and -20
°C for establishing the Creep Compliance Master Curve (CCMC). For
each design asphalt mixture at each temperature, 3 cylindrical
specimens with 150 mm in diameter and 50 mm in thickness are
prepared, so a total of 27 specimens are tested. As showed in
Figure 12, two strain gauges with a length of 38.1 mm were placed
at the center of the specimen to measure vertical and horizontal
deformations during loading.

Figure 12. Layout of Strain Gauges for SuperPave IDT Specimen
(Birgisson et al., 2007)

4.2.1 Resilient Modulus Test

The resilient modulus is a measure of a material’s elastic
stiffness. The ratio of the applied stress to recoverable strain
under applied repeated loads is known as resilient modulus. The
test is conducted in load control model by applying a repeated
haversine waveform load to specimen for a 0.1 second followed by
0.9 seconds rest period resulting in horizontal strain within the
range of 200 to 300 micro-strains. The resilient modulus is
calculated using the following equation:

MR = P ×GL H ×h×d× Ccomp

[19]

19

Ccomp = 0.6345 X Y − 1 − 0.332 [20]

where MR is resilient modulus, P is maximum load, GL is gauge
length, H is horizontal deformation, h is thickness of specimen, d
is diameter of specimen and Ccomp is

non-dimensional creep compliance factor, X Y is ratio of horizontal
to vertical deformation.

4.2.2 Creep Compliance Test

As creep compliance is a function of time-dependent strain over
stress so the time-dependent behavior of asphalt mixture can be
represented by the creep compliance master curve. Thus, it can be
used to evaluate the rate of damage accumulation of asphalt
mixture. The creep compliance test is carried out by applying a
constant load for 1000 seconds resulting in horizontal strain
within the range of 200 to 750 micro-strains. If the horizontal
deformation is greater than 180 micro-inches at 100 seconds, the
load is immediately removed from the specimen and then the specimen
is allowed to recover for a minimum 3 minutes before reloading at a
lower level.

Three parameters (D0, D1 and m-value) will be obtained from creep
compliance test. D0 describes the instantaneous elastic response,
D1 describes the initial portion of the creep compliance curve,
while m-value expresses the long-term portion of the curve. An
asphalt mixture with a low m-value exhibits a low rate of damage
accumulation.

4.2.3 Tensile Strength Test

The tensile strength test is conducted to determine the strength
and strain of the specimen in a displacement control model by
applying a constant rate of 50.8 mm/min until the specimen fails.
With the stress strain response, the dissipated creep strength
energy (DCSEf) is determined by deducting from fracture energy (FE)
to elastic energy (EE). Fracture energy is the area under the
stress strain curve to the failure strain. The tensile strength is
calculated as:

St = 2PCsx πdh

[21]

where St is indirect tensile strength, P is load of specimen, d is
diameter of specimen, h is thickness of specimen and Csx is
horizontal stress correction factor.

Csx = 0.948 − 0.0114 h d − 0.2693ν+ 1.436 h

d ν [22]

20

where Poisson’s ratio ν = 0.1 + 1.480 X Y 2 − 0.778 h

d 2 X Y 2 , X

Y is ratio of horizontal to

vertical deformation.

4.3 Thermal Stress Restrained Specimen Test

Thermal Stress Restrained Specimen Test (TSRST) was developed under
SHRP A-400 contract by Jung and Vinson (1994), which can be used to
evaluate the low-temperature cracking susceptibility of asphalt
mixture. As shown in Figure 13 and 14, the equipment comprises of
three subsystems: a cooling system, a load/displacement system, and
a test control/data acquisition system. In TSRST, the specimen is
subjected to thermal stress due to the decrease of temperature.
During the cooling process, the length of the specimen is held
constant so the specimen is restrained from shrinkage. As the
specimen contracts, two linear variable differential transducers
(LVDTs) sense the movement and a signal is sent to the computer,
which in turn causes the screw jack to stretch the specimen to its
original length. As the temperature continues to decrease, the
thermal stress increases until the specimen breaks. The temperature
at which the specimen fails is called fracture temperature and the
corresponding thermally induced stress is fracture stress.

Figure 13. Specimen Alignment Stand of TSRST

In Figure 15, a typical TSRST result with the obtained test
parameters is shown. At the beginning of the test, a relatively
slow increase in thermal stress is observed due to relaxation of
asphalt mixture. However, below the transition temperature, the
thermally induced stress is

21

linearly related to temperature. At the transition temperature, the
sample changes from a viscoelastic to elastic state. The transition
temperature and the slope of the stress-temperature curve, /, below
the transition temperature, may play an important role in
characterizing the rheological behavior of the asphalt mixture at
cold temperature.

Figure 14. Schematic of TSRST Apparatus (OEM Inc.)

Figure 15. Typical Stress versus Temperature Curve of TSRST (OEM
Inc.)

For each design asphalt mixture, 4 beam specimens (38 mm × 38 mm ×
200 mm) are prepared. In total, 12 specimens are tested in this
project. The tests are performed according

to AASTHO TP-10-93 specification, the specimen is pre-cooled at 2°C
for h before the test began, the initial temperature is 2 °C and
the cooling rate is 10 °C/h.

22

5 Data Analysis

To be a reliable and accurate thermal cracking model, it should be
able to provide clearly expected results. For example, a higher
thermal contraction coefficient should accelerate crack development
of asphalt mixture. In this chapter, the output results of the HMA
fracture mechanics-based thermal cracking model, such as the
predicted thermally induced stress and fracture temperature, will
be compared with the fracture stress and fracture temperature
obtained from TSRST, to finally evaluate the low temperature
cracking prediction of the model.

5.1 SuperPave IDT and TSRST Data

As described in Chapter 4, the SuperPave IDT and TSRST were
designed in this project and the test results are presented in this
section. Table 3 shows the different parameters of the three design
asphalt mixtures collected from SuperPave IDT at different
temperatures (0 °C, -10 °C and -20 °C), which are served as the
input data of the model. More details about the Matlab software for
obtaining these parameters were specified by Du (2010). Figure 16
shows the thermally induced stresses of the three design asphalt
mixtures develop with the changing cooling temperatures, which
basically match the typical TSRST result illustrated as Figure
15.

Table 3. Model Input Parameters Obtained from SuperPave IDT

Temp D0 D1 St FE DCSEf 0C 1/GPa 1/GPa MPa KJ/m3 KJ/m3

0 0,054 0,031 0,546 3,832 2,450 2,049 2,956 -10 0,038 0,010 0,477
4,112 1,172 0,837 5,192 -20 0,032 0,004 0,425 4,483 0,779 0,450
10,281 0 0,057 0,070 0,653 3,344 4,045 3,707 1,537

-10 0,041 0,014 0,547 3,856 0,820 0,510 1,663 -20 0,033 0,005 0,440
3,394 0,581 0,391 7,505 0 0,071 0,086 0,669 3,030 3,246 2,912
0,979

-10 0,052 0,026 0,644 3,451 1,372 1,050 1,195 -20 0,040 0,010 0,497
3,767 1,059 0,769 4,582

Mix-160-220

Figure 16. Stress versus Temperature Curve of TSRST

5.2 Creep Compliance Master Curve and Relaxation Modulus

Figures (17 – 22) show the different creep compliance data and the
Creep Compliance Master Curves (CCMC) fitted by power law for each
of the three design asphalt mixtures, respectively. The model
horizontally shifts the data obtained at various temperatures to
establish a smooth, continuous curve which is the CMCC at the
reference temperature (-20 °C), then the CCMC is fitted with power
model (cf. Equation [5]). Since the mathematical deficiency of
power law under multiple temperature ranges, the different
deviations are observed between the CCMCs and the power law fitted
curves.

0

0,5

1

1,5

2

2,5

3

3,5

4

4,5

T he

rm al

ly In

du ce

d St

re ss

, M Pa

Temperature, oC

24

Figure 17. Different Creep Compliance Data at Various Temperatures
for Mix-35-50

Figure 18. Creep Compliance Master Curve Fitted by Power Law for
Mix-35-50

25

Figure 19. Different Creep Compliance Data at Various Temperatures
for Mix-70-100

Figure 20. Creep Compliance Master Curve Fitted by Power Law for
Mix-70-100

26

Figure 21. Different Creep Compliance Data at Various Temperatures
for Mix-160-220

Figure 22. Creep Compliance Master Curve Fitted by Power Law for
Mix-160-220

27

Figure 23. Relaxation Modulus Fitted by Prony Series for
Mix-35-50

Figure 24. Relaxation Modulus Fitted by Prony Series for
Mix-70-100

28

Figure 25. Relaxation Modulus Fitted by Prony Series for
Mix-160-220

Figures (23 – 25) show the relaxation modulus fitted by Prony
Series for each of the three design asphalt mixtures, respectively.
Governing by the convolution integral (cf. Equation [6]), the creep
compliance and the relaxation modulus are clearly related by the
following curves. Also the relaxation modulus master curves for the
generalized Maxwell model are perfectly expressed by the Prony
series (cf. Equation [8]).

5.3 Thermally Induced Stress with Constant Thermal Contraction
Coefficient

With constant thermal contraction coefficients, Figures (26 – 37)
show the comparisons of the thermally induced stresses predicted by
the HMA fracture mechanics-based thermal cracking model (cf.
Equation [9]) and the stresses collected from TSRST. It can be
easily seen that the predicted stresses were quite close to the
observed stresses from TSRST for all samples, which indicate that
the HMA fracture mechanics-based thermal cracking model can provide
reasonable and reliable predictions for the thermal stress
development during the cracking process of HMA.

29

Figure 26. Comparison of Thermal Stress Using Two Methods for
Mix-35-50-1

Figure 27. Comparison of Thermal Stress Using Two Methods for
Mix-35-50-2

30

Figure 28. Comparison of Thermal Stress Using Two Methods for
Mix-35-50-3

Figure 29. Comparison of Thermal Stress Using Two Methods for
Mix-35-50-4

31

Figure 30. Comparison of Thermal Stress Using Two Methods
forMix-70-100-1

Figure 31. Comparison of Thermal Stress Using Two Methods for
Mix-70-100-2

32

Figure 32. Comparison of Thermal Stress Using Two Methods for
Mix-70-100-3

Figure 33. Comparison of Thermal Stress Using Two Methods for
Mix-70-100-4

33

Figure 34. Comparison of Thermal Stress Using Two Methods for
Mix-160-220-1

Figure 35. Comparison of Thermal Stress Using Two Methods for
Mix-160-220-2

34

Figure 36. Comparison of Thermal Stress Using Two Methods for
Mix-160-220-3

Figure 37. Comparison of Thermal Stress Using Two Methods for
Mix-160-220-4

35

5.4 Fracture Temperature

To accurately evaluate the HMA fracture mechanics-based thermal
cracking model, every sample’s predicted fracture temperature is
compared with the corresponding value collected from the TSRST.
According to Table 4, with constant thermal contraction
coefficients, the fracture temperatures predicted by the model have
evident divergences with the TSRST results. As a comparison, the
average fracture temperature predictions of the same three design
asphalt mixtures using the non-linear thermal contraction
coefficient are showed in Table 5.

It can be clearly seen that the variances of all three design
asphalt mixtures dramatically decrease in Table 5, which indicate
that the non-linear thermal contraction coefficient is more
suitable than the constant α value on predicting fracture
temperature. The comparison also demonstrates that the accuracy of
the fracture temperature prediction is greatly depends upon the
thermal contraction coefficient. More details about using no-linear
thermal contraction coefficient for fracture temperature prediction
were specified by Das et al. (2011).

Table 4. Comparisons of Fracture Temperatures with constant
contraction coefficient

Predicted TSRST Variance 0C 0C %

Mix-35-50-1 -20,05 -22,20 9,70 Mix-35-50-2 -20,00 -23,23 13,89
Mix-35-50-3 -23,54 -23,98 1,80 Mix-35-50-4 -23,23 -23,53 1,24

Avg. Mix-35-50 -21,71 -23,23 6,56 Mix-70-100-1 -19,27 -25,70 25,03
Mix-70-100-2 -19,62 -25,33 22,52 Mix-70-100-3 -20,58 -26,50 22,34
Mix-70-100-4 -21,13 -28,35 25,46

Avg. Mix-70-100 -20,15 -26,47 23,87 Mix-160-220-1 -29,29 -36,35
19,43 Mix-160-220-2 -25,91 -34,93 25,81 Mix-160-220-3 -23,83 -30,85
22,74 Mix-160-220-4 -25,20 -33,78 25,39

Avg. Mix-160-220 -26,06 -33,98 23,30

Sample ID

Predicted TSRST Variance 0C 0C %

Avg. Mix-35-50 -22,80 -22,00 -3,64 Avg. Mix-70-100 -23,60 -26,50
10,94

Avg. Mix-160-220 -27,70 -32,00 13,44

Mixture ID

5.5 Effect of Thermal Contraction Coefficient

In this section the fracture temperatures and fracture time
predicted by the HMA fracture mechanics-based thermal cracking
model using the different constant thermal contraction coefficients
are analyzed. For the Mix-70-100 and Mix-160-220, Table 6 and
Figures (39 – 40) clearly show that the higher thermal contraction
coefficient was applied, the higher fracture temperature and the
less fracture time the sample fails at. For the Mix-35-50, there
are a few exceptions of either fracture temperature or fracture
time, which may be due to the faults of data collection during the
TSRST where the thermal contraction coefficient originally deducted
from. However, the predicted fracture temperature and fracture time
do not vary too much from the expected ranges, so these data are
mostly in accordance with the expected results.

Figures (38-40) also clearly show the predicted 100-mm cracking
development versus time in the three design asphalt mixtures. In
the most fracture times, the damages increase at a relatively slow
rate. The crack lengths increase when the total accumulated DCSE
reaches DCSEf or the total accumulated FE reaches FE limit in the
every process zone. Since the newer process zones are always weaker
than the earlier zones due to the prolonged DCSE accumulated from
the beginning, the cracks grow at increasingly fast rates (i.e.
fewer number of loading cycles cause failure in the new process
zone) until the samples fail.

37

Table 6. Fracture Temperature and Fracture Time versus Thermal
Contraction Coefficient

Fracture Temperature Fracture Time Thermal Contraction Coefficient
0C Sec e-5/0C

Mix-35-50-1 -20,05 8900 3,13 Mix-35-50-2 -20,00 9000 3,06
Mix-35-50-3 -23,54 10600 2,00 Mix-35-50-4 -23,23 10200 1,84

Mix-70-100-1 -19,27 7800 5,88 Mix-70-100-2 -19,62 8000 5,45
Mix-70-100-3 -20,58 8300 4,99 Mix-70-100-4 -21,13 8400 4,92
Mix-160-220-1 -29,29 13100 4,46 Mix-160-220-2 -25,91 11200 6,39
Mix-160-220-3 -23,83 10200 8,01 Mix-160-220-4 -25,20 10800
6,96

Sample ID

0

20

40

60

80

100

120

3,13e-5/°C 3,06e-5/°C 2,00e-5/°C 1,84e-5/°C

Time (sec)

C ra

ck L

en gt

h (m

0

20

40

60

80

100

120

5,88e-5/°C 5,45e-5/°C 4,99e-5/°C 4,92e-5/°C C

ra ck

L en

gt h

(m m

C ra

ck L

en gt

h (m

6 Summary and Conclusion

The HMA fracture mechanics model is based on the theory of
viscoelasticity and energy-based fracture mechanics, which deals
with fracture associated with a fundamental dissipated creep strain
energy loss in viscoelastic materials. The TCMODEL developed based
on the theory of linear viscoelasticity is a proper
mechanistic-empirical design tool to predict thermal cracking in
asphalt pavement. In this project, the HMA fracture mechanics-based
thermal cracking model developed by Das et al. (2011) was studied.
Linear viscoelasticity from the TCMODEL, thermally induced
dissipated creep strain energy threshold and fracture energy
threshold were used to investigate low temperature cracking
performance. SuperPave IDT test results were used to compute
thermally induced stress and fracture temperature.

In experimental design, 27 SuperPave IDT specimens were tested at
different temperatures (0 °C, -10 °C and -20 °C) and then the
different parameters were input in the HMA fracture mechanics-based
thermal cracking model to step by step calculate the thermally
induced stresses, dissipated creep strain energy, fracture energy
and crack length. The data analysis of the thermal stresses and
fracture temperatures gained from the model and the TSRST
respectively were conducted and led to the following
findings:

• The model-predicted thermally induced stresses match well with
observed TSRST stress, which means the basic physics of
viscoelastic stress generated with temperature change is properly
followed.

• Thermal contraction coefficient is the key parameter for thermal
cracking performance prediction. By comprising the predicted
results which used the constant thermal contraction coefficient and
the no-linear thermal contraction coefficient, the model is
observed to be able to predict more accurate fracture temperatures
with the no-linear thermal contraction coefficient.

• The data analysis of the model-predicted crack length versus
fracture time validates that the higher thermal contraction
coefficient fastens the low temperature cracking development in
asphalt mixture.

• Since the new process zones are always weaker than the last zones
due to the prolonged DCSE accumulation, the cracks grow at
increasingly fast rates until the samples fail.

These conclusions indicated that this HMA fracture mechanics-based
thermal cracking model has the potential to reliably evaluate the
performance of asphalt mixtures subjected to thermally induced
damage. It is able to detect thermal stress with the changing
temperature and give an accurate output of crack development versus
temperature or time.

40

Future research area:

The findings of this study indicate that the HMA fracture
mechanics-based thermal cracking model has the potential to
reliably evaluate low temperature cracking resistance of asphalt
mixtures. However, this research needs to be continued to address
the following issues:

• Further study the performance of the model by testing the asphalt
mixture with polymer-modified binder.

• Applying different thermal contraction coefficients, e.g. linear
and bi-linear α values to evaluate the reliability and accuracy of
the model.

41

References

Birgisson, B., Montepara, A., Elena, R., Roque, R., and Tebaldi,
G., “The Effect of SBS Asphalt Modifier on Hot Mix Asphalt (HMA)
Mixture Cracking Resistance”, 4th International SIIV Congress,
Palermo, Italy, 2007.

Birgisson, B., Roque, R., Kim, J., and Pham, L.V., “The Use of
Complex Modulus to Characterize the Performance of Asphalt Mixtures
and Pavements in Florida”, Final Report for FDOT BD-273 Contract,
University of Florida, 2004.

Birgisson, B., Sangpetgnam, B., Roque, R., and Wang, J., “Numerical
Implementation of a Strain Energy-Based Fracture Model for a HMA
Materials”, International Journal of Road Materials and Pavement
Design, Vol. 8, Issue 1, 2007, pp. 7-45.

Birgisson, B., Sangpetgnam, B., Roque, R., and Zhang, Z., "Hot Mix
Asphalt Fracture Mechanics: A Fundamental Crack Growth Law for
Asphalt mixtures", Journal of the Association of Asphalt Paving
Technologists, Vol. 71, 2002, pp. 816-827.

Buttlar, W.G., Roque, R., and Hiltunen, D.R., “Prediction of
Thermal Cracking with TCMODEL”, Modeling of Asphalt Concrete, 2009,
pp. 405-427.

Buttlar, W.G., Roque, R., and Reid, B., “Automated Procedure for
Generation of Creep Compliance Master Curve for Asphalt Mixtures”,
Transportation Research Record, No. 1630, 1998, pp. 28-36.

Das, P.K., Jelagin, D., and Birgisson, B., “Low Temperature
Cracking Model Based on HMA Fracture Mechanics”, International
Journal of Solids and Structures, Under review, 2011.

Du, G.L., “Implementation of the SuperPave IDT Analysis Procedure”,
Master Degree Project, KTH Royal Institute of Technology,
Stockholm, 2010.

Hiltunen, D.R., and Roque, R., “A Mechanics-Based Prediction Model
for Thermal Cracking of Asphaltic Concrete Pavements”, Journal of
the Association of Asphalt Paving Technologists, Vol. 63, 1994, pp.
81-117.

Jung, D.H., and Vinson, T.S., “Low Temperature Cracking: Test
Section”, SHRP-A-400 Project Report, Strategic Highway Research
Program of National Research Council, Washington D.C., 1994.

Kim, J., Roque, R., and Birgisson, B., “Integration of Thermal
Fracture in the HMA Fracture model”, Journal of the Association of
Asphalt Paving Technologists, Vol. 77, pp. 631–661, 2008.

42

Nam, K., and Bahia, H.U., “Effect of Binder and Mixture Variables
on Glass Transition Behavior of Asphalt Mixtures,” Journal of the
Association of Asphalt Paving Technologists, Vol. 73, pp. 89–120,
2004.

National Cooperative Highway Research Program (NCHRP), “Evaluation
of Indirect Tensile Test (IDT) Procedures for Low-Temperature
Performance of Hot Mix Asphalt”, NCHRP Project Report 530,
Transportation Research Board of the National Academies, Washington
D.C., 2004.

OEM Inc., “Thermal Stress Restrained Specimen Test (TSRST) User’s
Manual”, Strategic Highway Research Program of National Research
Council SHRP-A-003A, Washington D.C..

Roque, R., Birgisson, B., Drakos, C., and Dietrich, B.,
“Development and Field Evaluation of Energy-Based Criteria for
Top-down Cracking Performance of Hot Mix Asphalt”, Journal of the
Association of Asphalt Paving Technologists, Vol. 73, 2004, pp.
229-260.

Tasdemir, Y., Das, P.K., and Birgisson, B., “Determination of
Mixture Fracture Performance with the Help of Fracture Mechanics”,
9th International Congress on Advances in Civil Engineering,
Trabzon, Turkey, 2010.

Vägverkt (Swedish National Road Administration), “ATB VÄG 2004
(General Technical Construction Specifications for Roads)”,
Available:
http://www.trafikverket.se/Foretag/Bygga-och-underhalla/Vag/Tekniska-dokument/Vagtek
nik/Aldre-versioner-av-ATB-Vag/ATB-Vag-2004/, Accessed 10 October
2011.

Witczak, M.W., Roque, R., Hiltunen, D.R., and Buttlar, W.G.,
“Superpave Support and Performance Models Management”, NCHRP 9-19
Project Report, 2000.

Zhang, Z., Roque, R., Birgisson, B., and Sangpetngam, B.,
“Identification and Verification of a Suitable Crack Growth Law”,
Journal of the Association of Asphalt Paving Technologists, Vol.
70, 2001, pp. 206-241.

43

Appendix

Code of Final.m

testdata=load('stress-35-50-1.txt'); % data from TSRST (Temp. vs
Stress)

data=load('35-50.txt'); % Data from IDT (Temp.,Do, D1, m)

%% Loading Data from Input files

temp=data(1:end,1);

ST=data(1:end,6); % Tensile strength from IDT test in MPa

DCSE_test=data(1:end,7); %DCSEf from IDT test in KJ/m3

time=[1;5;10;20;50;100;200;500;1000];

nn=7;

nm=7;

[reducedtime,CCredtim,aT2,aT3]=shifting(D0,D1,m,time,nn,nm);

[cf_,R,C,Coe]=relaxmodelAG2MW(t,Et);

t1 = -1/C(6);

t2 = -1/C(7);

t3 =-1/C(8);

t4 =-1/C(9);

t5 =-1/C(10);

[ljk,Et]=relaxation(ljk,crpcom,mvalue);

hold on

EE=E1*exp(-t./t1)+E2*exp(-t./t2)+E3*exp(-t./t3)+E4*exp(-t./t4)+E5*exp

(-t./t5);

loglog(t,EE,'g+')

Series',4)

eta=1000/(D1(3)*m(3)*(1000)^(m(3)-1));

% stress calculation by integrating normally by int. the shift
factor

time_T=(TSRST_Temp(1)-TSRST_Temp(end))*3600/coolingrate;

TSRST_T=(0:step:time_T)'; %generating same size of matrix as TSRST
time

aT=[0,aT2,aT3];

T=[-20,-10,0];

[Alpha]=alphatopu(aT,T,TSRST_stress,TSRST_T,E1,E2,E3,E4,E5,t1,t2,t3,t

gtext(titleStr);

figure;plot(time,stress,'r*')

z=5; %zone size

St=ST(3); % tensile srength from IDT test data

[fracture_time,crack_length,Fracture_Temp]=

crackgrowth(n,a,z,alpha,stress,ttr,eta,DCSE_test,temp,St,TT,time,FE_t

est)

end

end

46

end

end

figure

plot(time,CC0,'-.r*')

redtime2=logtime-aT2;

aT3=aT2+aT31;

% LINEARFIT(X,Y)

% Creates a plot, similar to the plot in the main curve
fitting

% window, using the data that you provide as input. You can

% apply this function to the same data you used with cftool

% or with different data. You may want to edit the function
to

48

%

% X = X:

% Y = Y:

f_ = clf;

legh_ = []; legt_ = {}; % handles and text for legend

xlim_ = [Inf -Inf]; % limits of x axis

ax_ = axes;

set(ax_,'Box','on');

X = X(:);

Y = Y(:);

'LineStyle','none', 'LineWidth',1,...

'Marker','.', 'MarkerSize',12);

xlim_(1) = min(xlim_(1),min(X));

xlim_(2) = max(xlim_(2),max(X));

if all(isfinite(xlim_))

set(ax_,'XLim',xlim_)

else

end

[cf_,R]= fit(X(ok_),Y(ok_),ft_);

C = coeffvalues(cf_);

Coe=coeffnames(cf_);

if 0

set(h_(1),'Color',[1 0 0],...

% Done plotting data and fits. Now finish up loose ends.

hold off;

h_ = legend(ax_,legh_,legt_,leginfo_{:}); % create legend

A=log10(redtime);

B=log10(fCC);

hold off

[cf,a]=curvefitting(A,B);

jk=[A(1):.1:A(end)]';%Reduce time in a constant interval of 0.4 in
log

scale

AAA=10.^AA;%D(t) in normal scale

ljk=10.^jk;%reduced time in normal scale

figure

50

loglog(ljk,AAA,'r*')

figure

%% Calculating m-value from fitted curve by
D(t)=Do+D1*t(red)^m

[cfinfo,xy,yy]=powerlaw(ljk,AAA);

mvalue=xy(2);

hold off

% CURVEFITTING(A,B)

% Creates a plot, similar to the plot in the main curve
fitting

% window, using the data that you provide as input. You can

% apply this function to the same data you used with cftool

% or with different data. You may want to edit the function
to

% customize the code and this help message.

%

% X = A:

% Y = B:

% X = A:

% Y = B:

f_ = clf;

legh_ = []; legt_ = {}; % handles and text for legend

xlim_ = [Inf -Inf]; % limits of x axis

ax_ = axes;

set(ax_,'Box','on');

A = A(:);

B = B(:);

% This dataset does not appear on the plot

% Add it to the plot by removing the if/end statements that
follow

% and by selecting the desired color and marker

if 0

h_ = line(A,B,'Color','r','Marker','.','LineStyle','none');

xlim_(1) = min(xlim_(1),min(A));

xlim_(2) = max(xlim_(2),max(A));

end % end of "if 0"

% --- Plot data originally in dataset "B vs. A (smooth)"

sm_.y2 = smooth(A,B,0.25,'lowess',0);

'LineStyle','none', 'LineWidth',1,...

'Marker','.', 'MarkerSize',12);

xlim_(1) = min(xlim_(1),min(A));

xlim_(2) = max(xlim_(2),max(A));

% Nudge axis limits beyond data limits

if all(isfinite(xlim_))

set(ax_,'XLim',xlim_)

else

end

cf_ = fit(A(ok_),sm_.y2(ok_),ft_);

aa = coeffvalues(cf_);

bb=coeffnames(cf_);

if 0

set(h_(1),'Color',[1 0 0],...

% Done plotting data and fits. Now finish up loose ends.

hold off;

set(h_,'Units','normalized');

53

% POWERLAW(LJK,AAA)

% Creates a plot, similar to the plot in the main curve
fitting

% window, using the data that you provide as input. You can

% apply this function to the same data you used with cftool

% or with different data. You may want to edit the function
to

% customize the code and this help message.

%

% X = ljk:

% Y = AAA:

f_ = clf;

legh_ = []; legt_ = {}; % handles and text for legend

xlim_ = [Inf -Inf]; % limits of x axis

ax_ = axes;

set(ax_,'Box','on');

ljk = ljk(:);

AAA = AAA(:);

'LineStyle','none', 'LineWidth',1,...

'Marker','.', 'MarkerSize',12);

xlim_(1) = min(xlim_(1),min(ljk));

xlim_(2) = max(xlim_(2),max(ljk));

if all(isfinite(xlim_))

set(ax_,'XLim',xlim_)

else

54

end

cf_ = fit(ljk(ok_),AAA(ok_),ft_,'Startpoint',st_);

xy= coeffvalues(cf_);

yy=coeffnames(cf_);

if 0

set(h_(1),'Color',[1 0 0],...

% Done plotting data and fits. Now finish up loose ends.

hold off;

set(h_,'Units','normalized');

% RELAXMODEL (T,ET)

% Creates a plot, similar to the plot in the main curve
fitting

% window, using the data that you provide as input. You can

% apply this function to the same data you used with cftool

% or with different data. You may want to edit the function
to

% customize the code and this help message.

% Number of datasets: 1

% Number of fits: 1

% X = t:

% Y = Et:

f_ = clf;

xlim_ = [Inf -Inf]; % limits of x axis

ax_ = axes;

set(ax_,'Box','on');

t = t(:);

Et = Et(:);

'LineStyle','none', 'LineWidth',1,...

'Marker','.', 'MarkerSize',12);

xlim_(1) = min(xlim_(1),min(t));

xlim_(2) = max(xlim_(2),max(t));

if all(isfinite(xlim_))

set(ax_,'XLim',xlim_)

else

fo_ = fitoptions('method','NonlinearLeastSquares','Lower',[0 0
0

0 0 -Inf -Inf -Inf -Inf -Inf],'Upper',[Inf Inf Inf Inf Inf 0 0
0

0 0]);

end

-0.006894 -0.00094280000000000004 -5.9200000000000002e-005

set(fo_,'Startpoint',st_);

ft_ =

fittype('a1*exp(b1*x)+a2*exp(b2*x)+a3*exp(b3*x)+a4*exp(b4*x)+a5*exp(b

5*x)',...

'b5'});

[cf_,R]= fit(t(ok_),Et(ok_),ft_,fo_);

C = coeffvalues(cf_);

Coe=coeffnames(cf_);

if 0

set(h_(1),'Color',[1 0 0],...

% Done plotting data and fits. Now finish up loose ends.

hold off;

[cf_,R,C,Coe]=linearfit(X,Y);

si=size(TSRST_T);

strain_rate=alpha*coolingrate/3600;

ttr=reducedtime(end)-reducedtime;

t=ttr;

E_tr=E1*exp(-t./t1)+E2*exp(-t./t2)+E3*exp(-t./t3)+E4*exp(-t./t4)+E5*e

xp(-t./t5);

58

figure;

si=size(tim);

figure,plot(tim,reducedtime,'--r')

ttr=reducedtime(end)-reducedtime;

t=ttr;

E_tr=E1*exp(-t./t1)+E2*exp(-t./t2)+E3*exp(-t./t3)+E4*exp(-t./t4)+E5*e

xp(-t./t5);

figure;loglog(t,E_tr,'r*')

%y_final=trapz(tim(1:end),I);

DCSE_next=DCSE_final(end,2:end);

FE_next=FE_final(end,2:end); %DCSE for adding up to the next
crack

%% n-th crack

nnn=n-ii; %number of zone

topu=[topu;kk];

Mode=[Mode,check];

Azz=cumsum(topu);

Az=Azz(end);

[DCSEnorm,kk]=crackgrowthDCSE_n(nnn,aaa,z,stress,ttr,eta,DCSE_test,dc

DCSE_next=DCSE_final(end,2:end); %DCSE for adding up to the next
crack

FE_final=FEnorm(1:(kk+1),:); %taking value upto FE_limit

FE_next=FE_final(end,2:end); %FE for adding up to the next
crack

%frc_tim=[frc_tim;frac_time];

crack_l=[crack_l;aaa];

ss=size(stress);

si=ss(2);

r=[];

end

sig=[];

sigma2=[St,sigma1]; %adding the St as the first value

sig=[sig;sigma2]; % finally the stress distribution

end

%--------------------------------------------------------------------

sigmaAVE=[sigmaAVE,sigmaAVE1];

zx=ttr./eta;

b=size(zx);

end

dcse=[];

DCSE=[];

DCSE=[DCSE,DCSE1];

dcse=[dcse,DCSE1'];

%--------------------------------------------------------------------

DE1=DCSE_test(1:2);

T1=temp(1:2);

X=T1;

Y=DE1;

[cf_,R,C,Coe]=linearfit(X,Y);

figure;

figure;

close

% geting data from the fitted curve (above and below -10C nad
-20C)

ww=size(TT);

nm=ww(1);

de2=E(1)*tem+E(2);

de3=C(1)*tem+C(2);

dcseref=DCSE_test(3); %DCSE limit at ref. Temp (-20C).

factor=dcseref./dcselimt;

topp=DE(:,ii);

DCSEnor1=DE(:,ii).*factor'; %Multiplying with factor in each column
of

dcse

64

jk=DCSEnor(:,1);

h=size(jk);

DE_f=[];

% info--> DCSE_nor-e je sokol value DCSE_f-er cheye boro, sei
gula-k alada

% korar 1ta loop

for ii=1:1:h(1)

ss=size(stress);

si=ss(2);

r=[];

end

sig=[];

sigma2=[St,sigma1]; %adding the St as the first value

65

end

%--------------------------------------------------------------------

sigmaAVE=[sigmaAVE,sigmaAVE1];

strain_th=alpha*(TT(1)-TT);

FE=[];

fe=[fe;FE1];

FE=[FE,FE1];

%

%
%------------------------------------------------------------------

FE1=FE_test(1:2);

figure;

figure;

close

% geting data from the fitted curve (above and below -10C nad
-20C)

ww=size(TT);

nm=ww(1);

de2=E(1)*tem+E(2);

de3=C(1)*tem+C(2);

feref=FE_test(3); %DCSE limit at ref. Temp (-20C).

factor=feref./felimt;

for ii=1:n

FEnor1=FE(:,ii).*factor'; %Multiplying with factor in each column
of dcse

FEnor=[FEnor,FEnor1];

jk=FEnor(:,1);

h=size(jk);

FE_f=[];

% info--> FE_nor-e je sokol value FE_f-er cheye boro, sei gula-k
alada

% korar 1ta loop

for ii=1:1:h(1)

n=nnn;

a=aaa;

ss=size(stress);

r=[];

end

sig=[];

sigma2=[St,sigma1]; %adding the St as the first value

sig=[sig;sigma2]; % finally the stress distribution

end

%--------------------------------------------------------------------

sigmaAVE=[sigmaAVE,sigmaAVE1];

zx=ttr(Az:end)./eta;

b=size(zx);

end

69

dcse=[];

DCSE=[];

DCSE=[DCSE,DCSE1];

%--------------------------------------------------------------------

% DCSE normalization:

% geting data from the fitted curve (above and below -10C nad
-20C)

dcseref=DCSE_test(3); %DCSE limit at ref. Temp (-20C).

factor=dcseref./dcselimt;

column of dcse

DCSEnorm=[];

jk=DCSEnorm(:,1);

h=size(jk);

DE_f=[];

% info--> DCSE_nor-e je sokol value DCSE_f-er cheye boro, sei
gula-k alada

% korar 1ta loop

for ii=1:1:h(1)

% %frac_time=time(kkk); %Corresponding time to grow the crack

% DCSE_next=DCSE_final(end,2:end); %DCSE for adding up to the next
crack

Code of crackgrowthFE_n.m

function[FEnorm,kk]=crackgrowthFE_n(nnn,aaa,z,stress,alpha,FE_test,fe

n=nnn;

a=aaa;

ss=size(stress);

si=ss(2);

r=[];

end

sig=[];

sigma2=[St,sigma1]; %adding the St as the first value

71

end

%--------------------------------------------------------------------

sigmaAVE=[sigmaAVE,sigmaAVE1];

strain_th=alpha*(TT(1)-TT);

zx=time(Az:end);

b=size(zx);

fe=[];

fe=[fe,FE1];

%--------------------------------------------------------------------

% DCSE normalization:

% geting data from the fitted curve (above and below -10C nad
-20C)

feref=FE_test(3); %DCSE limit at ref. Temp (-20C).

factor=feref./felimt;

column of dcse

FEnorm=[];

jk=FEnorm(:,1);

h=size(jk);

FE_f=[];

% info--> FE_nor-e je sokol value FE_f-er cheye boro, sei gula-k
alada

% korar 1ta loop

for ii=1:1:h(1)

% %frac_time=time(kkk); %Corresponding time to grow the crack